Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

No Downloads

Total views

331

On SlideShare

0

From Embeds

0

Number of Embeds

7

Shares

0

Downloads

7

Comments

0

Likes

1

No embeds

No notes for slide

- 1. CE305c127&128.doc University of New Mexico Civil Engineering Department Civil Engineering Materials Laboratory, CE 305L SPECIFIC GRAVITY & ABSORPTION OF COARSE & FINE AGGREGATES ASTM C127 & C128ScopeTest method C127 covers the determination of specific gravity and absorption of coarse aggregate. The specificgravity may be expressed as bulk specific gravity, saturated-surface-dry bulk specific gravity (SSD), or apparentspecific gravity.Test method C128 covers the determination of bulk, SSD specific gravity, and apparent specific gravity, andabsorption of fine aggregate. The bulk and apparent specific gravity are defined according to ASTM E12, whileabsorption is defined in ASTM C125.ReferencesASTM C127 Specific Gravity and Absorption of Coarse AggregateASTM C128 Specific Gravity and Absorption of Fine AggregateASTM E12 Definitions of Terms Relating Density and Specific Gravity of Solids, Liquids, and GasesASTM C125 Terminology Relating to Concrete and Concrete AggregatesASTM C29 Unit Weight and Voids in AggregateASTM C566 Total Moisture Content of Aggregate by DryingDefinitionsSpecific Gravity - the ratio of the mass (or weight) in air of a unit volume of material to the mass of the samevolume of water at a specified temperature. Specific gravity is a dimensionless term.Apparent Specific Gravity - the ratio of the weight in air of a unit volume of the impermeable portion of aggregateto the weight in air of an equal volume of gas-free distilled water at specified temperature.Bulk Specific Gravity - the ratio of the weight in air of a unit volume of aggregate (including the permeable andimpermeable voids in the particles, but not including the voids between particles) to the weight in air of an equalvolume of gas-free distilled water at specified temperature.Bulk Specific Gravity (SSD) - the ratio of the weight in air of a unit volume of aggregate, including the weight ofwater within the voids filled to the extent achieved by submersion in water for 24 hour (but not including the voidsbetween particles) to the weight in air of an equal volume of gas-free distilled water at specified temperature.Absorption - the increase in the weight of aggregate due to water in the pores of the material, but not includingwater adhering to the outside surface of the particles, expressed as a percentage of the dry weight. Dry aggregate isachieved when all uncombined water has been removed at a temperature of 110 C. 1
- 2. CE305c127&128.docASTM C127 (Coarse Aggregate)ApparatusScale (or balance)Sample Container (wire basket)Water TankSieves (No. 4)Drying OvenMaterialsCoarse Aggregate (>No. 4 sieve, i.e., gravel) - soaked for 24 hour, then saturated-surface-dried (SSD)Coarse Aggregate - Oven dried at 110 C, then cooled to room temperature.Note: The same gravel sample is used for both the SSD and oven dried states.Procedure1) Sieve dry material and reject all material finer than a number four sieve.2) Obtain approximately 3 kg of the water soaked material and roll it in a large absorbent cloth until all visiblefilms of water are removed. Wipe large particles individually as required to achieve a SSD condition. Weigh thetest sample in his SSD condition to the nearest 0.5 g or 0.05% of the sample weight, whichever is greater.3) Subsequently, place this SSD sample in the sample container and determine its weight in water. Be sure to tareout the sample container (wire basket) prior to placing the sample. Remove all air before weighing by shaking thebasket while immersed.4) Dry the sample to constant weight in an oven at 110 C, then allow to cool to room temperature. Weigh this drysample of coarse aggregate.5) Calculate the following: a) Bulk Sp. Gr. = A/(B-C) b) Bulk Sp. Gr. (SSD) = B/(B-C) c) Apparent Sp. Gr. = A/(A-C)where: A = weight of oven dried test sample in air, g B = weight of SSD sample in air, g C = weight of saturated sample in water, g.Express the above three values in terms of density, i.e., multiply the above calculated values by the density of waterat 4 C (62.43 lb/ft3).6) Calculate the percentage of absorption as follows: Absorption, % = [(B-A)/A] *100 2
- 3. CE305c127&128.docReport1) Report specific gravity results to the nearest 0.001.2) Report corresponding densities to the nearest 0.1 lb/ft3.3) Report the absorption to the nearest 0.1%. 3
- 4. CE305c127&128.docASTM C128 (Fine Aggregate)ApparatusScale (2 kg)Pycnometer - A flask or other suitable container into which the fine aggregate test sample can be readily introduced and in which the volume content can be reproduced within 0.1 cm3.Mold - A metal mold in the form of a frustum of a cone with dimensions of 40 mm top diameter, 90 mm bottom diameter, and 75 mm height.Tamper - A metal tamper weighing 340 g and having a flat circular tamping face of 25 mm diameter.Drying OvenMaterialsFine Aggregate (<No. 4 sieve, i.e., sand) - soaked for 24 hourFine Aggregate - Oven dried at 110 C, then cooled to room temperature.Note: The same sand sample is used for both the SSD and oven dried states.Procedure1) Obtain approximately 1 kg of the water soaked material by the following process. Decant excess water from thepan in which the fine aggregate has been soaking, being careful to avoid loss of fines.2) Spread sample on a flat nonabsorbent surface exposed to a gently moving current of warm air, stirringfrequently to ensure uniform drying.3) Follow the cone test for surface moisture, subsequently described; this cone test determines whether or notsurface moisture is present on the fine aggregate particles. The first trial of the cone test must be made with somesurface water present in the sample. Continue drying with constant stirring of the sample and cone tests atfrequent intervals until the cone test indicates that the fine aggregate has reached a saturated-surface-dry condition.4) Cone Test - Place mold, large side down, on a dry nonabsorbent surface. Place a portion of the partially driedsample loosely in the mold by filling it to overflowing. Lightly tamp the sample into the mold with 25 light dropsof the tamper (each drop should start about 5 mm (0.2 in.) above the top surface of the aggregate). The tampershould free fall under gravity during each drop. Distribute the 25 drops over the surface of the sample. Removeloose sand from around the outside base and lift the mold vertically. If surface moisture is still present, the sandcone will retain its molded shape. When the molded shape slightly slumps, a saturated-surface-dry condition hasbeen reached.5) Partially fill the pycnometer with water. Immediately introduce 500 g of saturated-surface-dry fine aggregateprepared as above. Record the weight of this SSD fine aggregate placed in the pycnometer. Fill the pycnometer to90% of capacity. Roll, invert, and agitate the pycnometer to eliminate all air bubbles (this can take 15 to 20 min).Bring the pycnometer to its calibrated capacity. Determine the total weight of the pycnometer, specimen, andwater. Note: Use distilled gas-free water in the pycnometer.6) Remove the fine aggregate from the pycnometer and dry to constant weight in an oven at 110 C, then cool toroom temperature, and weigh.7) Determine the weight of the pycnometer filled to its calibration capacity with water.8) Calculate the following: 4
- 5. CE305c127&128.doc a) Bulk Sp. Gr. = A/(B+S-C) b) Bulk Sp. Gr. (SSD) = S/(B+S-C) c) Apparent Sp. Gr. = A/(B+A-C)where: A = weight of oven dried test sample in air, g B = weight of pycnometer filled with water to calibration mark, g S = weight of SSD sample in air, g (prior to placement in pycnometer) C = weight of pycnometer with specimen and water to calibration mark, g.Express the above three values in terms of density, i.e., multiply the above calculated values by the density of waterat 4 C (62.43 lb/ft3).5) Calculate the percentage of absorption as follows: Absorption, % = [(S-A)/A] *100Report1) Report specific gravity results to the nearest 0.001.2) Report corresponding densities to the nearest 0.1 lb/ft3.3) Report the absorption to the nearest 0.1%.Questions1) Why is % Absorption important?NOTEThe following inequality must be satisfied for absorbing aggregates:Bulk Specific Gravity ≤ Bulk Specific Gravity (SSD) ≤ Apparent Specific Gravity 5

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment